- Nano Express
- Open Access
Enhanced electron transportation of PF-NR2 cathode interface by gold nanoparticles
Nanoscale Research Lettersvolume 14, Article number: 261 (2019)
In order to achieve a wider organic light-emitting diode (OLED) commercial popularity, solution processing inverted polymer light-emitting diode (iPLED) is a trend for further development, but there is still a gap for solution processing devices to achieve commercialization. The improvement of the performance iPLEDs is a research topic of intense current interest. The modification of the cathode interface layer of poly[(9,9-bis(3′-(N,N-dimethylamino)propyl)-2,7-fluorene)-alt-2,7-(9,9-dioctylfluorene)] (PF-NR2) can greatly improve the performance of the devices. However, the electron transportation of the cathode interface layer of PF-NR2 films is currently poor, and there is substantial interest in improving its electron transportation to further enhance the performance of organic optoelectronic devices. In this paper, gold nanoparticles (Au NPs) with a particle size of 20 nm were prepared and doped into the interface layer PF-NR2 at a specified ratio. The electron transportation of the interface layer of PF-NR2 was greatly improved, as judged by conductive atomic force microscopy measurements, which is due to the excellent conductivity of Au NPs. Herein, we demonstrate improved electron transportation of the interface layer by doping Au NPs in PF-NR2 film, which provides important and practical theoretical guidance and technical support for the preparation of high performance organic optoelectronic devices.
In the past two decades, organic light-emitting diodes (OLEDs) have attracted wide attention and been studied extensively due to their advantages of flexibility/bendability, diverse material design, easy synthesis and processing, low cost, and light weight. In particular, OLED displays and lighting have begun to realize industrialization and enter the market. Preparation of devices by a solution processing method can reduce the cost and is simple to implement [1,2,3,4,5,6,7]. In the past few years, the inverted polymer light-emitting diodes (iPLEDs) have been developed to enhance the stability and rectification ratio. However, there is still a large gap from commercialization for iPLEDs, and the improvement of the performance and life of the devices have become an important topic in current research and depends on the active layer material and interface of the device. In this type of device, charge is directly injected (or extracted) from the electrode to the organic semiconductor layer. Most active layer materials are p-type semiconductors, the number of holes is considerably higher than that of electrons, and high-efficiency devices require carrier injection (or extraction) and transport balance. This requires not only further structural design and modification of the luminescent material, but also methodological improvements in device preparation. Therefore, the properties of the cathode interface layer between the organic active layer and the interface electrode are critical. Therefore, it is necessary to improve the electrical properties of the cathode interface during device preparation [8, 9]. In this type of cathode interface layer, poly[(9,9-bis(3′-(N, N-dimethylamino)propyl)-2,7-fluorene)-alt-2,7-(9,9-dioctylfluorene)] (PF-NR2) is a representative cathode interface modification layer. It has also been previously reported to improve device performance by modifying the PF-NR2 interfacial layer. For example, Huang et al. carried out the addition of an epoxide to PF-NR2 side chains, so that they could undergo a crosslinking reaction on the surface of indium tin oxide (ITO) to enhance the electron transfer. The resulting iPLEDs with the polymer-poly(2-(4-(3′,7′-dimethyloctyloxyphenyl)-1,4-phenylene-vinylene)) (P-PPV) as the light-emitting layer gave a high luminous efficiency of 14.8 cd A−1 . Xie et al. enhanced the electron injection by modifying the PF-NR2 side chain to obtain an all-polymer white light-emitting device with a power efficiency of 11.4 lm W−1 . Chen et al. embedded K+ into the side chains at the interface layer to form a PFCn6:K+ structure, which effectively enhanced the interface conductivity and inhibited the recombination of electron-holes at the interface, so that the power conversion efficiency with poly(3-hexylthiophene): indene-C60 bisadduct (P3HT: ICBA) as the active layer was improved from 5.78 to 7.50% . Generally, the current modifications focusing on the cathode interface layer have all improved the material to enhance its carrier transportation, thereby improving the device performance.
Metal nanoparticles provide photoelectric properties that are available in many materials due to their special volume, quantum size, surface, and macroscopic quantum tunneling effects [13,14,15,16,17,18]. The performance of the device can be greatly improved by means that include surface-enhanced fluorescence, energy transfer, electrical effects, and scattering effects of metal nanoparticles. Therefore, the application of metal nanoparticles in optoelectronic devices has become a topic of significant interest [19,20,21,22,23,24,25,26,27,28,29,30,31,32,33]. In this paper, gold nanoparticles (Au NPs) with a particle size of 20 nm were prepared and doped into the interfacial layer of PF-NR2 at a specified ratio. Conductive atomic force microscopy (c-AFM) measurement showed that the electron transportation of the interface layer PF-NR2 was greatly improved. The results indicated that the doping of Au NPs into PF-NR2 could effectively improve the electron transportation of PF-NR2 film, which can be attributed to the excellent conductivity of Au NPs. The Au NPs/PF-NR2 hybrid film was preliminarily introduced into the inverted electroluminescent device, and the enhanced brightness ranged from 17 K cd m−2 to 33 K cd m−2 (94% improvement) and the luminous efficiency was increased from 9.4 cd A−1 to 18.9 cd A−1 (101% improvement). Herein, we investigated PF-NR2 on the surface of Au NPs to improve the electron transportation of the interface layer. The preparation process was simple and efficient, which provides an important and practical theoretical guidance and technical support for the preparation of high-performance iPLEDs.
Materials and Methods
The PF-NR2 synthesis process: 2,7-dibromo-9,9-bis(3-(N,N-dimethylamino)-propyl)fluorene (0.248 g, 0.500 mmol), 2,7-bis(4,4,5,5-tetramethyl-1,3,2-dioxaborolan-2-yl)-9,9-dioctylfluorene (0.321 g, 0.500 mmol), tetrakis (triph-enylphosphine)palladium [(PPh3)4Pd(0)] (10 mg), and several drops of Aliquat 336 were dissolved in a mixture of 3 mL of toluene and 2 mL of 2 M Na2CO3 aqueous solution. The mixture was refluxed with vigorous stirring for 3 days under an argon atmosphere. After the mixture was cooled to room temperature, it was poured into 200 mL of methanol. The precipitated material was recovered by filtration through a funnel. The resulting solid material was washed for 24 h using acetone to remove oligomers and catalyst residues (0.28 g, 77%).
P-PPV was purchased from Canton OLEDKING Optoelectric Materials Co., Ltd., Guangzhou, China. ITO glass substrates (size 15 × 15 mm ITO) were purchased from China Southern Glass Holding Corp, Shenzhen, China. Poly(3,4-ethylenedioxythiophene):poly(styrene-sulfonate) (PEDOT:PSS, Clevios P AI4083) was bought from Bayer AG.
Preparation of the Zinc Oxide (ZnO) Precursor
The ZnO precursor was prepared by dissolving zinc acetate dihydrate (Aldrich, 99.9%, 1 g) and ethanolamine (FuYu Fine Chemical Reagent Co., Ltd., 0.28 g) in 2-methoxyethanol (FuYu Fine Chemical Reagent Co., Ltd., 10 mL) under vigorous stirring for 12 h for hydrolysis in air [34, 35].
Synthesis of Au NPs
The Au NPs used here (20-nm diameter size) were synthesized according to the Frens method . A 100 ml sample of aqueous HAuCl4 (0.25 mM, Sinopharm Chemical Reagent Co., Ltd.) was prepared in a 250-ml flask. The solution was brought to boil while being vigorously stirred, with 1 mL of 5% aqueous trisodium citrate dihydrate (Enox) subsequently added. The reaction lasted 15 min until the solution reached a wine red color, indicating the Au NPs of desired size had been synthesized.
iPLED Device Fabrication
The ZnO precursor solution was spin-coated at 4000 r min−1 on top of the ITO-glass substrate. The films were annealed at 200 °C for 1 h in air. The ZnO film thickness was approximately 30 nm. The ZnO-coated substrates were then transferred into a nitrogen-filled glovebox. The PF-NR2 interlayer material was dissolved in methanol in the presence of a small amount acetic acid (10 μl ml−1), and its solution (concentration = 2 mg ml−1) was spin-coated on top of the ZnO film. P-PPV was dissolved into p-xylene with a concentration of 6 and 12 mg mL−1, respectively. The P-PPV films were prepared by spin-coating the solution at 1400 r min−1 solution onto the buffer layer with a thickness of approximately 80 nm. The pre-devices were then pumped down into vacuum (3 × 10−4 Pa). A 10-nm layer of molybdenum oxide (MoO3) was thermally deposited on top of the P-PPV layer at an evaporation rate of 0.1 Å s−1. Ultimately, a 120-nm Al film was deposited on top of the MoO3 layer through a shade mask. The overlap between the cathode and anode defined a 16.0 mm2 pixel area. Except for the deposition of the ZnO layers, all other processes were carried out in a controlled atmosphere of nitrogen in a glovebox (Vacuum Atmosphere Co.) containing less than 10 ppm oxygen and moisture.
Characterization of Devices and Thin Films
Conductive Atomic Force Microscopy
The conductivity was tested by Bruker-INNOVA. Conductive atomic force microscopy measurements (Bruker Innova AFM system) were performed in contact mode with a 3 N m−1-platinum/iridium-coated silicon cantilever. During the entire scanning process, the setpoint was kept as 1 V. This proper setpoint not only prevented the sample surface from being damaged during the repetitive scanning process, but also ensured the accuracy of the measurement. The local current value was measured by a current amplifier (Femto DLPCA-200) with a current gain of 107 V A−1.
Current density–voltage–brightness (I-V-B) characteristics were measured in the nitrogen glovebox using a Keithley 236 source measurement unit and a calibrated silicon photodiode. The UV-Vis spectra were recorded by a UV-3600 (SHIMADZU UV-3600). The film thickness was measured by a Dektak 150. The atomic force microscopy (AFM) images were recorded on a Seiko SPA 400 with an SPI 3800 probe station in tapping mode.
Results and Discussion
Characterization of Essential Properties of Au NPs and PF-NR2 Film
Au NPs with a particle size of 20 nm (TEM images in Fig. 1a) were prepared by the Frens method and dispersed in an aqueous solution. The absorption spectrum was measured, and its local surface-plasmon resonance (LSPR) peak was found at 520 nm (Fig. 1b). As judged by TEM image and the half peak width of in SPR, the synthesized Au NPs were uniform in size and well dispersed in aqueous solution, which is beneficial to the preparation of the device.
The solution of Au NPs and PF-NR2 (chemical structure shown in Fig. 2a) was uniformly mixed at an appropriate ratio (represented by PF-NR2/Au NPs), and PF-NR2 was prepared by the spin coating method . Because the thickness of the PF-NR2 film was too thin at a concentration of 0.5 mg L−1 and a speed of 2000 rpm and could not be accurately measured by a surface profilometer, we used a relatively thick PF-NR2 film for calibration based on the Lambert-Beer law [10, 37, 38], which states that the absorbance value is proportional to the film thickness (as shown in Fig. 2b). The absorbance value of the PF-NR2 film was 0.160 at a concentration of 2 mg L−1 and a speed of 1000 rpm, and the film thickness was measured to be 20 nm by surface profilometer. The absorbance value of a PF-NR2 film at a concentration of 2 mg L−1 and a speed of 2000 rpm washed by p-xy solution was 0.038, and the thickness of the PF-NR2 film was calculated to be 5 nm based on the Lambert-Beer law.
Both the PF-NR2 film and the PF-NR2/Au NP composite film were deposited on an ITO surface. The AFM characterization results of their surface morphologies are shown in Fig. 3a–c. The surface morphology of PF-NR2 was changed dramatically after the addition of Au NPs. As the hybrid layer consisted of PF-NR2/Au NPs, NPs were clearly observed in the AFM images for the hybrid layer, which showed a root mean square roughness (RMS) increase from 0.562 to 1.590 nm. The interfacial layers both with and without Au NPs are smooth surfaces, allowing high-quality polymer films to be fabricated onto its top. Phase contrast arises from compositional variations of the surface as well as the topographical variations . As seen in Fig. 3c, the phase contrast in PF-NR2/Au NPs can be reflected in its topography variation. Apparently, PF-NR2/Au NPs shows similar variation tendency in its height and phase images.
c-AFM Characterization of PF-NR2 Thin Films
In order to study the change in the electron transportation of the PF-NR2 film after adding Au NPs, we used c-AFM to determine the change in film conductivity. The schematic diagrams of the c-AFM measurements are shown in Fig. 4a–c. We used c-AFM to plot the I-V curves of PF-NR2/Au NPs with and without Au NPs shown in Fig. 4. At the same time, the electron-only device with the ITO/ZnO (30 nm)/PF-NR2 structure (5 nm, with and without Au NPs)/P-PPV (80 nm)/CsF (1.5 nm)/Al (120 nm) has been made to study the effect of Au NPs on electron transportation in Fig. 5. The current increased with the optimized concentration of the Au NPs in Figs. 4b and 5, which indicated that the Au NPs helps in electron injection. Electron transportation of the film with the presence of Au NPs was substantially improved due to the excellent electrical conductivity of the gold nanoparticles. Therefore, the addition of Au NPs to the PF-NR2 film can greatly improve the electron transportation of the interface layer. However, when the Au NPs reached a level of 120 pM, the conductivity of the film decreased. The reason might be that an excessively high concentration of Au NPs can cause an aggregation in the PF-NR2 film (The SEM image of without, 36 pM, 72 pM, and 120 pM Au NPs doping in PF-NR2 has been shown in Additional file 1: Figure S1), and the aggregated Au NPs will considerably reduce the electrical conductivity of the PF-NR2 film. We proposed a mechanism for the enhanced conductivity of the device by the Au NPs/PF-NR2 thin film, as shown in Fig. 6a. The introduction of Au NPs can improve the electron transportation of the PF-NR2 film, thereby enhancing the electron transport capability. Meanwhile, hole-transport is dominant in most polymer luminescent materials, so the improvement of electron transport performance can effectively improve the performance of the device.
In a device structure for general applications, the cathode interface layer will typically be in direct contact with the luminescent layer in iPLEDs. According to Förster energy transfer, if the Au NPs are directly in contact with the luminescent layer, the fluorescence would be quenched. Therefore, we measured the PL spectrum (Fig. 6c) of the luminescent layer based on P-PPV (chemical structure shown in Fig. 6b). As shown from the PL spectral results of the device, the introduction of Au NPs into the PF-NR2 film did not quench the fluorescence.
We preliminarily applied the PF-NR2/Au NP composite film to the iPLEDs with a device structure of ITO/ZnO (30 nm)/PF-NR2 (5 nm, with or without Au NPs)/P-PPV (80 nm)/MoO3 (10 nm)/Al (120 nm), the enhanced brightness ranged from 17 K cd m−2 to 33 K cd m−2 (94% improvement), and the luminous efficiency was increased from 9.4 cd A−1 to 18.9 cd A−1 (101% improvement), as shown in Fig. 7a–c. Based on our previous research conclusion, the weak improvement of PL intensity made little contribution to the device performance [19, 25]. The significant improvement in device performance indicates that Au NPs can improve the electron transportation of PF-NR2 and improve electron transport efficiency, thus enhancing the electron-hole recombination efficiency. With comprehensive consideration device efficiency, AFM phase imaging, and PL spectra, we conclude that the PF-NR2 film partially adhered to the surface of the Au NPs, which avoided direct contact of Au NPs with the luminescent layer P-PPV .
In this study, we prepared Au NPs with a size of about 20 nm by the Frens method, and the Au NPs were doped into the interface layer PF-NR2 at a specified ratio. It was found that the electron transportation of the interface layer PF-NR2 was effectively improved due to the excellent conductivity of Au NPs, while the interface layer of PF-NR2/Au NPs did not quench the fluorescence emission of the luminescent layer. Because most of the luminescent materials in devices are p-type semiconductors, the number of holes is substantially higher than that of electrons, and high-efficiency devices require carrier injection and transport balance. Therefore, improving the electron transportation of the cathode interface layer is a key method to effectively increase the efficiency of the device. Herein, an effective way to improve the electron transportation of the interface layer PF-NR2 by an Au NP interface doping was proposed, and the preparation process was simple and effective, which is important for preparing high-efficiency iPLEDs.
Availability of Data and Materials
The datasets used and/or analyzed during the current study are available from the corresponding author on reasonable request.
Atomic force microscopy
- Au NPs:
Brightness vs. current density
Conductive atomic force microscopy
Inverted polymer light-emitting diode
Indium tin oxide
Current density vs. applied voltage
Luminous efficiency vs. current density
Local surface plasmon resonance
Organic light-emitting diode
- P3HT: ICBA:
Poly(3-hexylthiophene): indene-C60 bisadduct
- PF-NR2 :
Polymer light-emitting diode
Transmission electron microscope
Choi H, Park JS, Jeong E, Kim GH, Lee BR, Kim SO, Song MH, Woo HY, Kim JY (2011) Combination of titanium oxide and a conjugated polyelectrolyte for high-performance inverted-type organic optoelectronic devices. Adv Mater 23:2759–2763
Yang X, Zhou G, Wong W-Y (2014) Recent design tactics for high performance white polymer light-emitting diodes. J Mat Chem C 2:1760–1778
Wang Q, Ma D (2010) Management of charges and excitons for high-performance white organic light-emitting diodes. Chem Soc Rev 39:2387–2398
Jiang Z, Zhong Z, Xue S, Zhou Y, Meng Y, Hu Z, Ai N, Wang J, Wang L, Peng J (2014) Highly efficient, solution processed electrofluorescent small molecule white organic light-emitting diodes with a hybrid electron injection layer. ACS Appl Mater Interfaces 6:8345–8352
Bolink HJ, Brine H, Coronado E, Sessolo M (2010) Ionically assisted charge injection in hybrid organic−inorganic light-emitting diodes. ACS Appl Mater Interfaces 2:2694–2698
Hu Z, Dong S, Xue Q, Xu R, Yip H-L, Huang F, Cao Y (2015) In-situ synthesis of metal nanoparticle-polymer composites and their application as efficient interfacial materials for both polymer and planar heterojunction perovskite solar cells. Org Electron 27:46–52
Chen H-W, Lee J-H, Lin B-Y, Chen S, Wu S-T (2018) Liquid crystal display and organic light-emitting diode display: present status and future perspectives. Light Sci Appl 7:17168
Lu LP, Kabra D, Johnson K, Friend RH (2012) Charge-carrier balance and color purity in polyfluorene polymer blends for blue light-emitting diodes. Adv Funct Mater 22:144–150
Peng J, Wang X, Liu J, Huang X, Xiao J, Wang S-D, Wang H-Q, Ma W (2014) A facile solution-processed alumina film as an efficient electron-injection layer for inverted organic light-emitting diodes. J Mater Chem C 2:864–869
Zhong C, Liu S, Huang F, Wu H, Cao Y (2011) Highly efficient electron injection from indium tin oxide/cross-linkable amino-functionalized polyfluorene interface in inverted organic light emitting devices. Chem Mater 23:4870–4876
Zhang B, Qin C, Ding J, Chen L, Xie Z, Cheng Y, Wang L (2010) High-performance all-polymer white-light-emitting diodes using polyfluorene containing phosphonate groups as an efficient electron-injection layer. Adv Funct Mater 20:2951–2957
Liao S-H, Li Y-L, Jen T-H, Cheng Y-S, Chen S-A (2012) Multiple functionalities of polyfluorene grafted with metal ion-intercalated crown ether as an electron transport layer for bulk-heterojunction polymer solar cells: optical interference, hole blocking, interfacial dipole, and electron conduction. J Am Chem Soc 134:14271–14274
Liu Y-L, Fang C-Y, Yu C-C, Yang T-C, Chen H-L (2014) Controllable localized surface plasmonic resonance phenomena in reduced gold oxide films. Chem Mater 26:1799–1806
Li Y-F, Feng J, Dong F-X, Ding R, Zhang Z-Y, Zhang X-L, Chen Y, Bi Y-G, Sun H-B (2017) Surface plasmon-enhanced amplified spontaneous emission from organic single crystals by integrating graphene/copper nanoparticle hybrid nanostructures. Nanoscale 9:19353–19359
Halas NJ, Lal S, Chang W-S, Link S, Nordlander P (2011) Plasmons in strongly coupled metallic nanostructures. Chem Rev 111:3913–3961
Rycenga M, Cobley CM, Zeng J, Li W, Moran CH, Zhang Q, Qin D, Xia Y (2011) Controlling the synthesis and assembly of silver nanostructures for plasmonic applications. Chem Rev 111:3669–3712
Su Y-H, Ke Y-F, Cai S-L, Yao Q-Y (2012) Surface plasmon resonance of layer-by-layer gold nanoparticles induced photoelectric current in environmentally-friendly plasmon-sensitized solar cell. Light Sci Appl 1:e14
Gu M, Li X, Cao Y (2014) Optical storage arrays: a perspective for future big data storage. Light Sci Appl 3:e177
Wu X, Liu L, Choy WC, Yu T, Cai P, Gu Y, Xie Z, Zhang Y, Du L, Mo Y (2014) Substantial performance improvement in inverted polymer light-emitting diodes via surface plasmon resonance induced electrode quenching control. ACS Appl Mater Interfaces 6:11001–11006
Choi H, Ko S-J, Choi Y, Joo P, Kim T, Lee BR, Jung J-W, Choi HJ, Cha M, Jeong J-R (2013) Versatile surface plasmon resonance of carbon-dot-supported silver nanoparticles in polymer optoelectronic devices. Nat Photonics 7:732
Wu X, Liu L, Yu T, Yu L, Xie Z, Mo Y, Xu S, Ma Y (2013) Gold nanoparticles modified ITO anode for enhanced PLEDs brightness and efficiency. J Mater Chem C 1:7020–7025
Ko S-J, Choi H, Lee W, Kim T, Lee BR, Jung J-W, Jeong J-R, Song MH, Lee JC, Woo HY (2013) Highly efficient plasmonic organic optoelectronic devices based on a conducting polymer electrode incorporated with silver nanoparticles. Energy Environ Sci 6:1949–1955
Wu X, Liu L, Deng Z, Nian L, Zhang W, Hu D, Xie Z, Mo Y, Ma Y (2015) Efficiency improvement in polymer light-emitting diodes by mitting di effect of gold nanoparticles. Part Part Syst Charact 32:686–692
Kim SH, Bae T-S, Heo W, Joo T, Song K-D, Park H-G, Ryu SY (2015) Effects of gold-nanoparticle surface and vertical coverage by conducting polymer between indium tin oxide and the hole transport layer on organic light-emitting diodes. ACS Appl Mater Interfaces 7:15031–15041
Wu X, Zhuang Y, Feng Z, Zhou X, Yang Y, Liu L, Xie Z, Chen X, Ma Y (2018) Simultaneous red–green–blue electroluminescent enhancement directed by surface plasmonic “far-field” of facile gold nanospheres. Nano Res 11:151–162
Wu X, Li Y, Wu L, Fu B, Liu G, Zhang D, Zhao J, Chen P, Liu L (2017) Enhancing perovskite film fluorescence by simultaneous near-and far-field effects of gold nanoparticles. RSC Advances 7:35752–35756
Wu X, Li Y, Li W, Wu L, Fu B, Wang W, Liu G, Zhang D, Zhao J, Chen P (2018) Enhancing optically pumped organic-inorganic hybrid perovskite amplified spontaneous emission via compound surface plasmon resonance. Crystals 8:124
Peng J, Xu X, Tian Y, Wang J, Tang F, Li L (2014) Improved efficiency in polymer light-emitting diodes using metal-enhanced fluorescence. Appl Phys Lett 105:1_1
Gu Y, Zhang D-D, Ou Q-D, Deng Y-H, Zhu J-J, Cheng L, Liu Z, Lee S-T, Li Y-Q, Tang J-X (2013) Light extraction enhancement in organic light-emitting diodes based on localized surface plasmon and light scattering double-effect. J Mater Chem C 1:4319–4326
Xiao Y, Yang J, Cheng P, Zhu J, Xu Z, Deng Y, Lee S, Li Y, Tang J (2012) Surface plasmon-enhanced electroluminescence in organic light-emitting diodes incorporating Au nanoparticles. Appl Phys Lett 100(8)
Chen P, Xiong Z, Wu X, Shao M, Meng Y, Xiong Z-H, Gao C (2017) Nearly 100% efficiency enhancement of CH3NH3PbBr3 perovskite light-emitting diodes by utilizing plasmonic Au nanoparticles. J Phys Chem Lett 8:3961–3969
He X, Wang W, Li S, Wang Q, Zheng W, Shi Q, Liu Y (2015) Localized surface plasmon-enhanced electroluminescence in OLEDs by self-assembly Ag nanoparticle film. Nanoscale Res Lett 10:468
Woo S, Jeong JH, Lyu HK, Han YS, Kim Y (2012) In situ-prepared composite materials of PEDOT: PSS buffer layer-metal nanoparticles and their application to organic solar cells. Nanoscale Res Lett 7:641
Liang J, Zhong W, Ying L, Yang W, Peng J, Cao Y (2015) The effects of solvent vapor annealing on the performance of blue polymer light-emitting diodes. Org Electron 27:1–6
Zheng H, Zheng Y, Liu N, Ai N, Wang Q, Wu S, Zhou J, Hu D, Yu S, Han S (2013) All-solution processed polymer light-emitting diode displays. Nat Commun 4:1971
Frens G (1973) Controlled nucleation for the regulation of the particle size in monodisperse gold suspensions. Nat Phys Sci 241:20
Zhong C, Duan C, Huang F, Wu H, Cao Y (2010) Materials and devices toward fully solution processable organic light-emitting diodes. Chem Mater 23:326–340
Ma H, Yip HL, Huang F, Jen AKY (2010) Interface engineering for organic electronics. Adv Funct Mater 20:1371–1388
Liu S, Yu H, Zhang Q, Qin F, Zhang X, Zhang L, Xie W (2019) Efficient ITO-free organic light-emitting devices with dual-functional PSS-rich PEDOT: PSS electrode by enhancing carrier balance. J Mater Chem C 7(18):5426–32
Liu F, Nunzi J-M (2011) Phosphorescent organic light emitting diode efficiency enhancement using functionalized silver nanoparticles. Appl Phys Lett 99:203
This research was funded by the National Natural Science Foundation of China, grant number 11602243, 11504300; NSFA of China, grant number U1630125.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. The SEM images of without, 36 pM, 72 pM, and 120 pM Au NP doping in PF-NR2. (DOCX 393 kb)